Supporting information without S1 Supporting Information Structures and magnetism...
Embed Size (px)
Transcript of Supporting information without S1 Supporting Information Structures and magnetism...
Structures and magnetism ofmono‐palladium and mono‐platinum doped Au25(PET)18 nanoclusters
Shubo Tian,a Lingwen Liao,a Jinyun Yuan,b Chuanhao Yao,a Jishi Chen, a Jinlong Yang, b
1Key Laboratory of Materials Physics, Anhui Key Laboratory of Nanomaterials and Nanotechnology, Institute of Solid State Physics, Chinese Academy of Sciences, Hefei 230031, China. Email: firstname.lastname@example.org. 2Hefei National Laboratory for Physical Sciences at the Microscale and Synergetic Innovation Center of Quantum Information and Quantum Physics, University of Science and Technology of China, Hefei, Anhui 230026, China 1. Experimental section
Reagents. All chemicals and reagents are commercially available and were used as received. The water used in all experiments was ultrapure (resistivity 18.2 MΩ cm), produced with a Milli‐Q NANO pure water system. Toluene (99.5%), methanol (AR), dichloromethane (AR), petroleum ether (AR) and Sodium borohydride (NaBH4, 99.0%), were purchased from Sinopharm chemical reagent co., ltd. Tetraoctylammonium bromide (TOAB, 98.0%), Sodium tetrachloropalladate (NaPdCl4, 98%) and Chloroplatinic acid hexahydrate (H2PtCl6∙4H2O) was obtained from Aladdin. 2‐Phenylethanethiol (PhC2H4SH, 99.0%) and 1‐hexanethiol (CH3(CH2)5SH, 99.0%) were purchased from Sigma‐Aldrich. Tetrachloroauric(III) acid (HAuCl4∙4H2O, 99.7%) were purchased from Shanghai chemical reagent co., ltd.
Synthesis of the anion and neutral Au25(SR)18. [Au25(PET)18]‐TOA+ was prepared via the previous method reported.1 [Au25(PET)18]0 was synthesized through the controlled oxidation of [Au25(PET)18]‐TOA+ by O2 in air.2 [Au25(SC6H13)18]0 was synthesized referring to the above methods.
Synthesis of [Au24Pd(PET)18]0 and [Au24Pt(PET)18]0. Both [Au24Pd(PET)18]0 and [Au24Pt(PET)18]0 nanoclusters were synthesized according to a reported method3,4,5 with some modifications.
The first step: H2PtCl6∙4H2O (0.1036 g, 0.20 mmol), HAuCl4∙4H2O (0.329g, 0.80 mmol) and TOAB (0.634 g, 1.16 mmol) were dissolved in 30 mL THF in a 125 mL tri‐neck round bottom flask. After vigorously stirred for 60 min, the solution color changed from yellow to red. Then, phenylethanethiol (0.345 mL) was added to the flask at room temperature without changing the stirring speed. Stirring was continued for 10 min until the solution color changed from dark red to orange. After that, NaBH4 (0.380 g, 10.0 mmol) dissolved in 5 mL cold water was added all at once. After stirred for additional 5 h, the aqueous phase was removed and the remaining
Electronic Supplementary Material (ESI) for Chemical Communications. This journal is © The Royal Society of Chemistry 2016
organic phase was washed with abundant water to remove water soluble impurities. Then the products in organic phase were precipitated out by the addition of CH3OH.
The second step: the crude products were dissolved in a small amount of CH2Cl2 then separated by preparative thin‐layer chromatography (dichloromethane: petroleum ether=2:3). The isolated mixture products of Au25(PET)18 and [Au24Pt(PET)18]0 were dissolved in 10 ml toluene and into the resulting solution 15 mL H2O2 (30 wt%) solution was added to selectively decompose the Au25(PET)18 nanoclusters. When the homo‐gold nanoclusters was completely decomposed after about 10 hours, the alloy nanoclusters were further purified using PTLC.
The third step: high qualified single crystals of [Au24Pt(PET)18]0 were obtained by slowly diffusing methanol into the toluene solution of the purified product at 4 °C for 5 days.
The first step of [Au24Pd(PET)18]0 synthesis is similar to that of [Au24Pt(PET)18]0 except using Na2PdCl4 (0.0589 g, 0.20 mmol) instead of H2PtCl6∙4H2O (0.1036 g, 0.20 mmol) as the second metal source; and the remaining protocols are also similar to those of [Au24Pt(PET)18]0 synthesis except that the etching time by H2O2 was adjusted to ~3 hours.
2. Characterization. The ultraviolet–visible–near‐infrared absorption spectra were measured on a UV‐2600 spectrophotometer (Shimadzu, Japan) at room temperature. Matrix‐assisted laser desorption ionization time of flight mass spectrometry (MALDI‐TOF‐MS) was performed on an autoflex Speed TOF/TOF mass spectrometer (Bruker) using Trans‐2‐[3‐(4‐tert‐Butylphenyl)‐2‐methyl‐2‐propenylidene] malononitrile (DCTB) as the matrix. The diffraction data for PdAu24(PET)18 and PtAu24(PET)18 were collected at 130K on a Bruker APEX DUO X‐ray diffractometer using Mo Ka radiation (λ = 0.71073). NMR spectra were recorded on an agilent spectrometer (VNMRS600) using tetramethylsilane as an internal reference. The Pt and Au L3‐edge XAFS spectra were measured at the 1W1B beamline of Beijing Synchrotron Radiation Facility (BSRF), China.
3. Theoretical method. In order to confirm the relative stability of the three isomers of Pt locating at core, inner‐shell and out‐shell for Au24Pt(PET)18, their single point energies were calculated using Density Functional Theory (DFT) with the hybrid functional B3LYP 6‐9 and all electron basis set 6‐31g (d, p) for H, C, and S, pseudopotential basis set LANL2DZ for Au and Pt, as implemented in the Gaussian 09 program package.10 These three isomers were constructed by placing the Pt atom in the core, inner‐shell, and outer‐shell of Au24Pt crystallized in this work, respectively.
4. REFERENCES 1. Wu, Z.; Suhan, J.; Jin, R. One‐pot synthesis of atomically monodisperse,
thiol‐functionalized Au25 nanoclusters. J. Mater. Chem. 2009, 19, 622‐626. 2. Zhu, M.; Eckenhoff, W. T.; Pintauer, T.; Jin, R. Conversion of anionic Au25(SCH2CH2Ph)18‐ cluster to charge neutral cluster via air oxidation. J. Phys. Chem. C 2008, 112, 14221‐14224. 3. Negishi, Y.; Kurashige, W.; Niihori, Y.; Iwasa, T.; Nobusada, K. Isolation, structure, and stability of a dodecanethiolate‐protected Pd1Au24 cluster. Phys. Chem. Chem. Phys. 2010, 12, 6219‐6225. 4. Qian, H.; Jiang, D.‐e.; Li, G.; Gayathri, C.; Das, A.; Gil, R. R.; Jin, R. Monoplatinum Doping of Gold Nanoclusters and Catalytic Application. J. Am. Chem. Soc. 2012, 134, 16159‐16162. 5. Kwak, K.; Tang, Q.; Kim, M.; Jiang, D‐e.; Lee, D. Interconversion between Superatomic 6‐Electron and 8‐Electron Configurations of M@Au24(SR)18 Clusters (M = Pd, Pt). J. Am. Chem. Soc. 2015. 137, 10833−10840. 6. A. D. Becke, Phys. Rev. A, 1988, 38, 3098–3100. 7. C. Lee, W. Yang and R. G. Parr, Phys. Rev. B: Condens. Matter, 1988, 37, 785–789. 8. A. D. Becke, J. Chem. Phys., 1993, 98, 5648–5652. 9. P. J. Stephens, F. J. Devlin, C. F. Chabalowski and M. J. Frisch, J. Phys. Chem., 1994, 98, 11623–11627. 10. Frisch, M. J. et al. Gaussian 09, Revision B.01 (Gaussian, Inc., 2010).
5. Supporting Figures
Figure S1 The ultraviolet–visible–near‐infrared spectra of [Au25(PET)18]‐, [Au25(PET)18]0, [Au25(SC6H13)18]0, Au24Pd(PET)18, Au24Pt(PET)18, Au25Ag2(PET)18, Au24Cd(PET)18 and Au24Hg(PET)18。
Figure S2 The matrix‐assisted laser desorption ionization mass spectra of [Au25(PET)18]‐, [Au25(PET)18]0, Au24Pd(PET)18 and Au24Pt(PET)18.
Figure S3 The total structure of [Au24Pd(PET)18]0.
Figure S4 The total structure of [Au24Pt(PET)18]0.
Figure S5 XANES of Pt foil and Au24Pt(PET)18 nanoclusters.
Figure S6 The illustration of (α‐ CH2)in, (α‐ CH2)out, (β‐CH2)in, and (β‐ CH2)out in Au25
Figure S7 The 1H NMR spectra of [Au25(PET)18]‐ (a), [Au25(PET)18]0 (b), [Au24Pd(PET)18]0
(c) and [Au24Pt(PET)18]0 (d). (2.5ppm‐6.0ppm)
Figure S8 The 1H NMR spectra of [Au25(PET)18]‐ (a), [Au25(PET)18]0 (b), [Au24Pd(PET)18]0 (c) and [Au24Pt(PET)18]0 (d).
Figure S9 The temperature‐dependent 1H NMR spectra of neutral [Au25(PET)18]0.
Figure S10 The 2D H‐H COSY NMR spectrum of